- Research article
- Open Access
The necessary length of carbon nanotubes required to optimize solar cells
© Vaezzadeh et al 2007
Received: 12 June 2007
Accepted: 01 October 2007
Published: 01 October 2007
In recent years scientists have been trying both to increase the efficiency of solar cells, whilst at the same time reducing dimensions and costs. Increases in efficiency have been brought about by implanting carbon nanotubes onto the surface of solar cells in order to reduce the reflection of sunrays, as well as through the insertion of polymeric arrays into the intrinsic layer for charge separation.
The experimental results show power rising linearly for intrinsic layer thicknesses between 0–50 nm. Wider thicknesses increase the possibility of recombination of electrons and holes, leading to perturbation of the linear behaviour of output power. This effect is studied and formulated as a function of thickness. Recognition of the critical intrinsic layer thickness can permit one to determine the length of carbon nanotube necessary for optimizing solar cells.
In this study the behaviour of output power as a function of intrinsic layer thicknesses has been described physically and also simulated. In addition, the implantation of carbon nanotubes into the intrinsic layer and the necessary nanotube length required to optimize solar cells have been suggested.
Developing inexpensive and renewable energy sources is one of the most important scientific and technological challenges of our time. Solar energy is an inexhaustible energy source that can be harnessed to meet our growing future energy needs. However, traditional photovoltaic (solar-to-electric conversion) technology is too expensive to be the suitable alternative for fossil fuels or even other competing renewable energy sources. A significant leap in the scientific and technological progress of renewable energy sources will be required to displace proven, but unsustainable energy production methods.
Nanotechnology is driving new interesting developments in photovoltaic technology. Advances in organic synthesis and characterization techniques allow us to coax a photocurrent from organic, 'soft' molecules in a process that mimics photosynthesis in plants, thus potentially opening up the way to cheap, ubiquitous solar cells. Power production resulting in zero greenhouse gas emissions is economically and environmentally desirable. Direct photovoltaic conversion of sunlight into electricity is therefore the highly attractive alternative to unsustainable energy sources such as fossil fuels.
Although silicon solar cells have gained a considerable market share and commercial success, high production and up-front installation costs still limit their commercial viability. In this study, we explore the use of low-cost advanced materials for photovoltaic energy production and the mechanism of photovoltaic action in a new class of solar cell, that is, the heterojunction photovoltaic. These are constructed from a thin film of cheap composite material, a mixture of carbon nanotubes and conductive polymer .
We will first discuss the results for illumination through the p-layer (solid symbols in the figure). For intrinsic layers that are sufficiently thin, the power is proportional to the number of photons absorbed (i.e. to the product of the thickness, d and the absorption coefficient, η). Within this limit the fill factors have nearly ideal values around 0.8. As the thickness of the cell increases, the power saturates. In figure 1 the first plot (η = 100 000/cm – corresponding photon energy of about 2.3 eV) shows the behaviour for strongly absorbed illumination. Power saturation occurs for thicknesses greater than 100 nm, that is, typical distance at which photons are absorbed. Since thicker cells do not absorb much additional light, going beyond this length means power stops increasing .
Model and objective
Different models have been proposed to simulate the experimental results [3–8]. Figure 1 shows the behaviour of power as a function of intrinsic layer thickness. Several experiments have been carried out to demonstrate the effect of layer thickness on output power.
As can be observed in figure 1, power grows linearly and becomes saturated after a distinct value of layer thickness. If we neglect recombination of electrons and holes, the output power can be expressed as:
P α = αw,
where, α is a coefficient and can be calculated for each curve, w is the intrinsic layer thickness, with Pα termed the ideal power (linear form).
On the basis of figure 2 we can produce an equation that contains the recombination phenomena as:
P = P α - β(w - wc) n ,
Figure 3 shows the ideal (linear form), theoretical and experimental powers as a function of the intrinsic layer thickness for P1 type. The recombination phenomena start at Wc = 40 nm, which we call the critical intrinsic layer.
From figure 3 it can be seen that the theoretical power values between 0–150 nm almost match the experimental results. However after 150 nm the agreement between the fits is poor. When the difference between the intrinsic layer thickness and carrier current cross section is small, the two-dimensional recombination phenomena are expected to dominate (from 40 nm up to 150 nm for P1 type). Whereas, when the difference between the intrinsic layer thickness and carrier current cross section is large (after 150 nm for P1 type) the three-dimensional recombination phenomena dominate. On increasing the length of intrinsic layer, the three-dimensional recombination becomes dominant and exhibits linear behaviour.
Therefore, the theoretical model plot can be defined by three regions that is, linear (0–40 nm), two-dimensional and three-dimensional recombination phenomena:
P = αw - β(w - wc) n + (a - α'w),
where a and α' are the three dimensional recombination coefficients.
Because of interference between two-dimensional and three-dimensional recombination terms in equation 3, this equation is not appropriate for simulation. Consequently we need to modify equation 3 thus:
P th = αw - β(|w - wc|) n X(w) + (a - α'w)Y(w),
where X (w) is the creation and destruction function and Y (w) is the creation function.
where γ is function sharpness parameter.
Data plotted for the calculation of theoretical power (γ = 5).
P1 (100 000/cm)
P2 (50 000/cm)
P3 (20 000/cm)
P4 (10 000/cm)
The necessary length of carbon nanotube for an optimized solar cell
Because of the symmetry and unique electronic structure of graphene, the nanotube's structure strongly affects its electrical properties. For a given (n, m) nanotube, if n – m is a multiple of 3, then the nanotube is metallic; such is the case for all armchair (n = m) nanotubes. In terms of metallic behaviour, carbon nanotubes can have conductivity up to eight times that of copper, and can carry a current density comparable to that of any known conventional metallic wire; this makes carbon nanotubes potential candidates as nanoscale wires . It is consequently possible to reduce the recombination phenomena by using the carbon nanotubes in the intrinsic layer. The presence of an aligned doped carbon nanotube (armchair, superconducting) in the intrinsic layer helps maintain linear power generation behaviour, in addition to making solar cells with higher output powers.
It is necessary to know the proper length of doped carbon nanotubes as a function of intrinsic layer thickness. The non-linearity of power starts at wc, which for P1 type, for example, starts at 40 nm. So the necessary length of carbon nanotube for optimizing a solar cell, as a function of the intrinsic layer, can be expressed as:
L nanotube = w - wc
It is important to note that the volume occupied by carbon nanotubes in the intrinsic layer affects only the linearity coefficient.
When considering the behaviour of power as a function of intrinsic layer thickness, the recombination of electrons and holes plays an important role in reducing the power. Eliminating recombination is useful in maintaining the linear behaviour of power and in producing solar cells with high powers. If the intrinsic layer thickness is comparable to the carrier current cross section, the two dimensional recombination phenomena are dominant; otherwise the three dimensional recombination phenomena would dominate. In this study, power as a function of the intrinsic layer thickness was simulated and plotted, thus allowing us to express the necessary length of carbon nanotubes required for optimized solar cells as a function of the intrinsic layer thickness.
- Motta N, Waclawik ER, Goh R, Bell JM: Nanotube-polymer Solar Cells – an Alternative to Silicon. Bollettino della Comunità Scientifica in Australasia. 2005, 15-20. [http://eprints.qut.edu.au]16
- Luque A, Hegedus S: John Wiley & Sons Handbook of Photovoltaic Science and Engineering. 2003, Ltd ISBN: 0-471-49196-9View ArticleGoogle Scholar
- Davis Mark, Hunter Fanney A, Dougherty Brian: Evaluating building integrated photovoltaic performance models. National Institute of Standards and Technology, Gaithersburg, MD. 20899, -8632Google Scholar
- Dianove M, Kazansky PG, Stepanovd Yu: Photovoltaic model of photoinduced second-harmonic generation in optical fibers. Acad Sci USSR. General physics inst., dep. fiber optics, Moscow 117942, URSS (Sov. lightwave commun.)Google Scholar
- De Blas MA, Torres JL, Prieto E, Garca A: Selecting a suitable model for characterizing photovoltaic devices. Renewable Energy. 2002, 25 (3): 371-380(10). 10.1016/S0960-1481(01)00056-8.View ArticleGoogle Scholar
- Cristofari C, Poggi P, Notton G, Muselli M: Thermal Modelling of a Photovoltaic Module. Proceeding Modelling, Simulation, and Optimization. 2006, 507:Google Scholar
- Hunter Fanney A, Dougherty Brian, Davis Mark: Short-Term Characterization of Building Integrated Photovoltaic Panels. National Institute of Standards and Technology. 2002, 100 Bureau Drive, MS 8632, Gaithersburg, MD 20899-8632Google Scholar
- Munoz-Perez MA, Rodriguez-Pichardo A, Camacho Martinez F, Sidrach-de-Cardona M, Mora Lopez L: A simple model for sizing stand alone photovoltaic systems. Solar Energy Materials and Solar Cells. 55 (3): 199-214(16). 24 August 1998Google Scholar
- Appenzeller J, Martel R, Derycke V, Radosavljevic M, Wind S, Neumayer D, Avouris P: Carbon nanotubes as potential building blocks for future nanoelectronics. Microelectronic Engineering. 2002, 64 (1-4): 391-7. 10.1016/S0167-9317(02)00813-4.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.